1 AN ABSTRACT OF THE THESIS OF Ronald W. Buckingham for the degree of Master of Science in Mechanical Engineering presented on March 2, 1993 Title: An Experimental Study on the Use of Inclusion Trapping Devices for Investment Casting Redacted for Privacy Abstract approved Dr. Lorin R. Davis A problem facing the casting industry is inclusions in the finished parts. The inclusions can be sand from the molds, oxides or other impurities in the metal charge. Inclusions lead to costly part repairing or reworking. A study was done to try and find inclusion trapping devices that could be placed in the gating system. The experiments consisted of pouring water and suitable inclusion models into clear, full scale, plastic molds. The fills were video taped for later analysis. The efficiency of the trapping device was determined from the end location of the inclusions. No work was done on other anti-inclusion methods such as ceramic filters, bottom pour ladles, chemical additives, etc. The research showed that a swirl chamber which used centrifugal force to separate inclusions worked quite well if set up correctly. The optimum setup was a vertical swirl chamber with a well. The inlet passage was choked and located below the exit passage. It also worked much better than any setup which tried to use buoyancy for separation. The large volume of the swirl chamber may be objectionable. However, properly shaped inserts, such as an ice-cream cone shape, can be put into the chamber to reduce fill volume while still maintaining good efficiency and fills Ṫhe efficiencies of the chambers behave as expected; faster pours are less efficient and bigger chambers (for a constant size mold) are more efficient. The use of outlet chokes may or may not improve separation efficiency, but will improve the filling of the part cavity.
2 An Experimental Study on the Use of Inclusion Trapping Devices for Investment Casting By Ronald W. Buckingham A THESIS submitted to Oregon State University in partial fulfillment of the requirements for the degree of Master of Science Completed March 2, 1993 Commencement June 1993
3 ACKNOWLEDGEMENTS I would like to thank my major professor, Dr. Lorin R. Davis, for his encouragement and guidance on this project. I would also like to thank Precision Castparts Corporation for their financial support and technical assistance that made this project possible.
4 APPROVED: Redacted for Privacy Professor of Mechanical Engineering in charge of major Redacted for Privacy Head of department of Mechanical Engineering Redacted for Privacy Dean of Graduat chool (I Date thesis is presented March 2, 1993 Typed by Ron Buckingham for Ronald W. Buckingham
5 TABLE OF CONTENTS I. INTRODUCTION 1 Investment Casting 1 Inclusions Encountered in Investment Casting. 3 Previous Work 3 II. EXPERIMENTAL WORK 9 Overall Setup 9 Inclusion Models 10 Equipment 12 Procedure 16 III. WORK DONE 19 Buoyancy Chambers 19 Small Swirl Chambers 23 Conical Swirl Chambers 25 Large Swirl Chamber 26 IV. RESULTS 27 Buoyancy Chambers 27 Small Swirl Chambers 32 Conical Swirl Chambers 51 Large Swirl Chambers 52 Miscellaneous Separaters 61 V. CONCLUSION 62 VI. BIBLIOGRAPHY 66 VII. APPENDICES 68 Appendix A: Raw data for all runs 68 Appendix B: Inclusion information 126
6 LIST OF FIGURES Figure Page 1. Typical buoyancy trap for sand casting Typical swirl chamber for sand casting Gating system insert 8 4. Gating system insert positioned in the mold 8 5. Crucible stand shown with small bucket crucible Small mold setup Large mold setup Mechanism to separate inclusions using buoyancy Buoyancy cylinder Various shaped chokes Small swirl chamber Conical swirl chambers Buoyancy chamber with offset inlet and exit Buoyancy cylinder with baffle Inlet vs. outlet location on swirl chamber Small swirl chambers; plain, well, extension and cap Small swirl chamber efficiency for slow pour Small swirl chamber efficiency for medium pour Small swirl chamber efficiency for fast pour Efficiency of plain swirl chamber with inlet choke. Slow pour Efficiency of plain swirl chamber with inlet choke. Medium pour Efficiency of plain swirl chamber with inlet choke. Fast pour Fill time of plain swirl chamber with inlet choke. Slow pour Fill time of plain swirl chamber with inlet choke. Medium pour Fill time of plain swirl chamber with inlet choke. Fast pour Efficiency of swirl chamber with inlet choke and 2" well. Slow pour Efficiency of swirl chamber with inlet choke and 2" well. Medium pour Efficiency of swirl chamber with inlet choke and 2" well. Fast pour Radial, tangential and anti-tangential outlets Large swirl chambers with clay and inserts Ice-cream cone shaped insert 60
7 LIST OF TABLES Table Page I. Effect of pour rate on heavy and light inclusion separation efficiency for a 3.5" dia X 3.75" horizontal cylinder using buoyancy for separation. (runs ) II. Effect of cylinder length on heavy and light inclusion separation efficiency for a 3.5" dia horizontal cylinder using buoyancy for separation. All pours medium speed. (runs , , ) 30 III Effect of overflow outlet choke on heavy and light inclusion separation efficiency for a 3.5" dia X 3.75" horizontal cylinder using buoyancy for separation. All pours medium speed. (runs , ) 30 IV. Effect of internal baffle on heavy and light inclusion separation efficiency for a 3.5" dia X 3.75" horizontal cylinder using buoyancy for separation. All pours medium speed. (runs , ) 32 V. Summary of results for small swirl chambers VI. Effect of venturi outlet choke on separation efficiency for small swirl chambers 45 VII. Fluid velocities in the 3" dia swirl chamber with 2" well 51 VIII. Summary of results for conical swirl chambers.. 52 IX. Summary of results for large swirl chamber X. Effect of outlet configuration on large swirl chamber separation efficiency 57 XI. XII. Effect of clay filler on separation efficiency for large swirl chamber with well and 50% inlet choke 58 Effect of insert 2 on separation efficiency for large swirl chamber with well and 50% inlet choke 59
8 An Experimental Study on the Use of Inclusion Trapping Devices for Investment Casting I. INTRODUCTION A problem facing the casting industry is inclusions in the finished parts. The inclusions can be sand from the molds, oxides or other impurities in the metal charge. Inclusions lead to costly part repairing or reworking. Many schemes for reducing inclusions in the part exist, including ceramic filters, bottom pour ladles, improved tundish designs, chemical additives, etc. However, the work done here was on devices that can be placed somewhere in the runner system to stop or separate the inclusions before they reach the part cavity. INVESTMENT CASTING Investment casting, sometimes called the lost wax process, attained industrial importance at the end of WW II for making rocket components and jet turbine blades from materials that are not readily machinable. A wax pattern of the desired part is constructed and attached to wax runners, gates and a downsprue and tundish. It is then dipped in a slurry and coated with sand. After this sets, the mold is heated, melting out the wax, leaving a hard ceramic mold. This is then preheated and filled with the desired metal. Although this form of casting is complex and expensive,
9 very intricate shapes can be cast, thin sections (0.015") can be made and tolerances can be kept to 0.005"-0.010". One important way that investment casting differs from sand casting is that the harder ceramic shell allows faster pouring rates. The faster pour rates are required to fill the smaller and more intricate parts of the mold cavity usually found in investment casting. These higher fluid velocities can lead to problems such as cold shots, cold shuts, nofill and ceramic wash. A cold shot occurs when a portion of the metal flow separates from the main flow, then solidifies and won't properly fuse back with the rest of the material. A cold shut is when two separate flows solidify and come together. They do not fuse properly leaving a lap line. Nofill is when a section of the mold does not get filled due to trapped gases or early solidification of the metal flow. Ceramic wash occurs when the fluid flow erodes the mold walls. This leads to inclusions in the metal flow and changes the shape of the mold. Besides ceramic wash, inclusions or other impurities can be present in the original metal charge. The purpose of this project was to find ways using flow 2 control devices in the gating system to remove or trap inclusions before they got into the part cavity.
10 3 INCLUSIONS ENCOUNTERED IN INVESTMENT CASTING A summary of inclusions that are encountered in investment casting was provided by Precision Castparts Corporation (PCC). For this experiment their alloys were divided into two groups; titanium alloys which have "heavy" inclusions and Ni-, Fe-, and Co-base alloys that have "light" inclusions. Titanium alloys have a density of 4.5 g/cma3 and the two common inclusion types have densities of 9.9 and 5.0 g/cma3, giving inclusions that are heavier than the alloy. The composition of these inclusions is not known since this information is proprietary. Ni-, Fe-, and Co-base alloys have higher densities than titanium, g/cma3. The common types of inclusions found are alumina, silica, mullite and oxides. These have densities ranging from 2.3 to 3.96 g/cma3, giving inclusions that are lighter than the alloy. A detailed list of these inclusions is given in the appendix. PREVIOUS WORK The study of investment casting has already been done at OSU in cooperation with PCC and the Oregon Metals Initiative (OMI). The work consisted of video taping water as it filled clear plastic or resin molds. Work was done in the area of flow modeling for centrifugal casting. This
11 is where the molds are rotated at high speeds while they are being filled to increase the "gravity" and fill the parts 4 quicker. Another study looked at the use of flow control devices to minimize turbulence and poor filling characteristics. These include waves, flow separation, splashing, flow reversal, bubbles and pumping of the fluid. The flow control devices were various shaped chokes in the gates and downsprue, wells, runner extensions and different shaped downsprues and runners. A numerical score was given to each pour based on the number and severity of bad fill characteristics. Other smaller projects have also been done. A filling technique was studied in which the mold tilted along with the crucible. The idea was to reduce turbulence in the downsprue much in the same way one tilts a glass and pours down the side from a bottle. PCC has made clear resin molds of some production molds in which they were experiencing fill problems. sent to OSU for study. These were A literature search was done at the beginning of the project. Much information was found on inclusions such as their chemical composition, where inclusoons comes from, and how to control them using bottom pour ladles, chemical additives, ceramic filters, or different foundry procedures.[6,7,8,9,10,11,12]
12 Very little information was found on inclusion traps, and all of the traps found were for sand casting, not 5 investment casting. Most of these traps used buoyancy to trap inclusions. Usually, the gate connecting the part cavity to the runner was smaller than the runner and attached low. The mechanism is the runner will fill and light inclusions will float to the top of it. Clean metal then goes into the gate. There were various shapes of this type of trap. Figure 1 shows a schematic of how these traps work. Figure 1. Typical buoyancy trap for sand casting There seems to be only two commonly used traps that use centrifugal force. relatively simple. The mechanism by which this works is Fluid enters a cylindrical vertical chamber tangentially causing a swirl to form. A resultant
13 centrifugal force pushes the lighter inclusions toward the center, and clean fluid is taken off the outside. Heavier inclusions sink to the bottom. The first commonly found swirl chamber was used in sand casting. Since sand cast parts cannot have undercuts (unless premade cores are used) the top of the inlet runner 6 and the bottom of the exit runner are in the same plane. Figure 2 shows a typical swirl chamber used in sand casting[14,15]. --> Side view Top view Figure 2. Typical swirl chamber for sand casting The other centrifugal trap was a prefabricated "whirlgate." This consisted of a central, vertical sprue channel surrounded by a spiral runner. The gating system
14 insert (figure 3) is assembled from individual, premade 7 ceramic flights stacked on top of each other. This insert is then placed at the bottom of the downsprue as shown in figure 4. The lighter inclusions are forced to the center and caught on the bottom of the inserts[16,17].
15 8 Figure 3. Gating system insert pouring basin gating system insert Figure 4. Gating system insert positioned in the mold
16 9 II. EXPERIMENTAL WORK OVERALL SETUP The casting process during this study was modeled by full size clear plastic molds and water. The fills were recorded with a video camera for analysis later. The use of water to model molten metal has already been largely justified by previous work done at OSU.(18] Water was chosen as the working fluid because it is safe, inexpensive, easy to photograph, and has a viscosity value that is similar to molten titanium. Unfortunately, water has the drawback that its surface tension and density vary significantly from most molten metals. All modeling in this system was done in full scale due to the variety of flows present in the mold. To have a properly scaled down model, one must maintain consistency between the model and the full scale version with respect to the Reynolds number, Froude number and Weber number. This requires either three different-sized models or a full sized model. The Reynolds and Froude numbers were satisfied rather well because of the similarity between the viscosity water and a molten alloy like titanium. However, the Weber number deviated greatly for the model because of differences between the densities and surface tensions of of the
17 10 water and molten metal. The idea of using water to model metal was tested earlier at OSU. first with water, similar conditions. A Pyrex mold was filled and videotaped then with a low melting solder under The results showed that the splashing and turbulence for the metal was less than for the water. This was attributed to the larger surface tension forces in the molten metal. However, after the initial splashing, the fills were very similar. The effect of vacuum vs. ambient pours was also investigated. Much of PCC's parts are poured in a vacuum to reduce oxidation. A vacuum chamber was constructed to compare different pairs of pours, one being poured in the vacuum and one being poured at ambient pressure. The results showed that there was little difference in the fluid flow and recommended that future tests be made at ambient pressure for simplicity. INCLUSION MODELS After a meeting with PCC engineers in April of 1991, emphasis shifted from heavy inclusions to light ones. They felt that this was the more important problem at present. They were still interested in heavy inclusions for titanium castings, however. From the summary of inclusions supplied by PCC, a list
18 11 was made of possible inclusion models. This list is given in the appendix. The studies have mainly centered around four inclusion models. Light Inclusions 3mm cubic wood beads, s.g. = mm round wood beads, s.g. = Heavy inclusions 3mm acetate balls, s.g. = 1.2 6mm glass balls, s.g. = 2 The 3mm size was the biggest that PCC was interested in. The bigger particles were sometimes used for better visibility on the videocamera. The use of many small particles was considered since this would give much better statistical results and be closer to the size that PCC wanted to study. However, they were messy to use and required filtering of the water after each run to determine where various particles went. Some runs were made with cork particles, bubble alumina, sandblasting medium and silica to check the larger inclusion models. results of the
19 EQUIPMENT 12 Most of the major equipment for studying inclusions was already in place, thanks to the previous work of Sewell and Miller. This included the crucible stand, hydraulic crucible controls, small mold stand, LSBO table (large mold stand), video camera, VCR, lighting and fixtures, video monitor, previous molds and parts, various extra plexiglass material and an assortment of tools. The crucible stand shown in figure 5 was a large structure built from steel I beams and square tubing by PCC. It had adjustable height and could support two types of crucibles; a tilting bucket type and a bottom pour type. The tilting bucket had a maximum volume of 9.7 liters and was used with the small molds. It was operated by the hydraulic crucible control. This used an electronically driven hydraulic pump to pressurize hydraulic oil. This activated a hydraulic cylinder connected to the crucible which would tip it. The hydraulic fluid was controlled by a needle valve. Adjusting this needle valve would then give pour rates that could be repeated. Three pour rates were used, slow (S), medium (M) and fast (F). For a pour volume of two liters, this corresponded to pour times of about 4 seconds, 2.5 seconds and 1.5 seconds respectively.
20 13 Crucible 7' 4" max 5' 6" min Height adjustment peg ' Figure 5. Crucible stand shown with small bucket crucible The bottom pour crucible was a 17 gallon drum with a hand operated gate valve on the bottom. It was used with the large LSBO mold. (LSBO stands for Large Structure Business Operations, a division of Precision Castparts Corp.) Different pour rates could be obtained by opening the gate valve to a specific place. For a pour volume of
21 6.7 gallons, the approximate pour times were 10 seconds (slow), 6 seconds (medium) and 1.4 seconds (fast). 14 The small mold consisted of a tundish, 1.5" diameter downsprue, a 1.5" diameter runner, the inclusion trapping device, a 1.125" diameter gate, and the part mold. These were all mounted on a 29" X 18" piece of 0.5" clear plexiglass which was attached to the mold stand. The setup was positioned so the tundish was underneath the tilting crucible. See figure 6. The part mold used was the one used in earlier studies for flow evaluations. tundish crucible vent 1.5" downsprue part cavity Plexiglas clear resin mold Inclusion Trapping Device drain plug 1.5' runner gate 29" Figure 6. Small mold setup
22 A large mold was used to check the scaleability of the 15 results. It consisted of a 3.5" downsprue, an 8" swirl chamber, four 2.5" outlet gates and four thin, square molds (approximately 12" X 10" X 5/8"). See figure 7. There was no tundish as the downsprue was connected directly with the bottom of the crucible. z17 gallon drum reservoir 1..L4,,,... Gate valve...",,,..-3.5" dia downsprue o 2.5" dia vent.5" Ma runner with 12" X 10" X 5/8" part mold - (typical) degrees from swirl chamber 8" dia X 14" (with well) large swirl chamber Figure 7. Large mold setup
23 A Panasonic AG-170 VHS videocamera was used to record the fills. The shutter speed was set to 1/500 which is 16 faster than normal. This lead to darker pictures, requiring additional background lighting. However, the faster shutter speed gave clearer pictures when viewed on slow play or pause. A shroud made of plastic sheeting with a plexiglass viewport was built to cover the camera during experiments. This was to protect the camera from unplanned water splashing. A Sony trinitron monitor and Panasonic AG-2510 VCR were also used to analyze the fills and make backup tapes. The monitor was used to better focus the video camera, the screen giving a better picture than the camera's small internal viewing screen. PROCEDURE The procedure for modeling the inclusion traps is summarized below. Initial setup of the mold; tundish, downsprue, runner(s), inclusion trap and part mold(s). The crucible was filled with the proper amount of water. Each run was identified with a number. Before the pour, the camera was turned on. The crucible was either poured or gate valve opened at the desired pour rate.
24 17 Inclusions were introduced to the fluid. The method depended on the particular setup and at what time the inclusions should be introduced. The fill was timed. The camera was turned off. A count of the inclusions location was made. at each critical The efficiency of the inclusion trap was based on the number of inclusions that got through the trap and the number of inclusions captured by the trap. Any inclusions that didn't make it to the trap (remained in tundish, downsprue or runner) were not used in efficiency calculation. There was no formal flow evaluation (for smoothness of mold filling) of each run as was done in previous work. The goal of this study was to find an inclusion trap that worked the best. Afterwards, if the flow in the runners or part mold was poor, it could be improved by using runner chokes or other techniques. This was the purpose of earlier work done at OSU. Another reason for not analyzing each flow was the sheer volume of them. Giving a numerical flow evaluation number to each pour was a long, tedious and somewhat arbitrary task. The number of inclusion runs was around This high number is due to two things. First, the nearly infinite number of possible inclusion trapping
25 geometries. Second, it was found early on that one run was 18 not enough to adequately find the efficiency of the trap. Usually, five identical runs were made with every setup to give a better statistical average. All flows are on video tape. They can be viewed by contacting the Department of Mechanical Engineering at Oregon State University.
26 III. WORK DONE 19 The work done can be roughly summarized below. Various configurations of the cylindrical separation chambers (which used buoyancy) were tested on the small mold. The 4", 3.5", 3" & 2.5" dia. swirl chambers were tested on the small mold with various configurations. Two cone shaped swirl chambers the small mold. Miscellaneous traps were tried mold. were tested on on the small An 8" dia. swirl chamber was tested on the large mold. This was to verify the small swirl chamber results and see effects of more runners and larger volumes. BUOYANCY CHAMBER Our studies began by investigating chambers which used buoyancy to trap inclusions. This chamber was a cylinder (3.5" I.D. X 3.75" long max) positioned horizontally with inlet and outlet passages on each end. Fluid would fill the chamber completely, then any light inclusions would float to the top and heavy inclusions would sink to the bottom.
27 20 Clean fluid would be taken off in the middle figure 8. as shown on light inclusions clean fluid 'b heavy inclusions Figure 8. Mechanism to separate inclusions using buoyancy The cylinder was adjustable as shown in figure 9. The endcaps were movable, so the effective length of the cylinder could be varied as well as the inlet's and outlet's relative position to each other. Various shaped chokes (figure 10) could be located at the inlet and/or exit. Internal baffles of various shapes could also be placed inside.
28 21 \optional baffl 3.5" die X 3.75" cylinder 1 <-----> Adjustable length // L1.5" dia inlet i 1.125" die outlet various endcaps baffle Figure 9. Buoyancy cylinder
29 22 overflow choke underfloor choke venturi choke Figure 10. Various shaped chokes Tests using the cylinders were done on the small mold. Usually, the small 3mm wood beads were used, but some tests used the larger wood beads for camera visibility. Tests using heavy inclusions were also done. The inclusions were introduced at various places and times during the pour.
30 23 Middle (M): inclusions were put in by hand at the top of the tundish when approximately half of the fluid was out of the crucible. Beginning (B): inclusions were put in by hand at the top of the tundish when the fluid just started to leave the tundish. Pre-Pour (PP): inclusions were placed at the bottom of the downsprue at the elbow before the fluid was poured. SMALL SWIRL CHAMBER During this experiment, four small swirl chambers were made with inside diameters of 2.5", 3", 3.5" and 4". These had inside heights of 3.5". The cylinders were made from sections and held together with clear tape so they were adjustable. The inlet passage could be above or below the exit. The exit passage could leave tangentially "with" the inlet fluid or "against" it (which we called antitangential). As shown in figure 11, wells, extensions and caps could easily be attached. the inlet and/or exit. Chokes could be placed at
31 24 ->p swirl chamber 8 4 side view choke locations spraelkii tangential exit anti-tangential exit Figure 11. Small swirl chamber The small swirl chambers were tested on the small mold, in the same way that the buoyant traps were done. The tests were nearly exclusively done with light inclusions, since the swirl chamber was specifically designed for them. Some testing was done with heavy inclusions for completeness. Nearly all inclusion introduction was pre-pour since that appeared to be the worst case and the best test of separators.
32 25 CONICAL SWIRL CHAMBERS Two cone shaped swirl chambers were cast from plastic resin. These are shown in figure 12. The inlets and outlets were the same size as used on the small swirl chambers (1.5" and 1.125" respectively). Cone 1 had two tangential exits, one of which was plugged with clay during testing. Cone 2 had a radial exit. Cone 1: 4" die base 10" high Cone 2: 4.7 die base 11" high Figure 12. Conical swirl chambers
33 26 LARGE SWIRL CHAMBER The later part of the work was on a large, 8" dia swirl chamber (see figure 7). The large swirl chamber was built to see if the results and trends of the smaller ones were consistent. One main difference in the large swirl chamber was the use of four outlets going to four part cavities, instead of just one. In a meeting with PCC in October of 1991, they expressed interest in a large swirl chamber that could feed parts radially. PCC already makes large circular parts such as turbines and nozzles. The downsprue is in the middle of the part, and runners feed off radially. They wanted something that could also be stuck in the middle of the part with a minimum amount of modification to their existing wax patterns. The part cavities attached to this swirl chamber are the ones used previously to model a mold for PCC's LSBO. Inclusions were introduced in two ways for the large swirl chamber. Usually, the light beads were put in a "basket" with the bottom made from window screen. This was then flipped over and placed at the bottom of the drum above the gate valve. For late inclusions, a small hole was drilled in the downsprue just above the elbow. A piece of tubing was connected to the hole and a large syringe. inclusions were then injected into the flow. The
34 27 IV. RESULTS The raw data for all runs are given in the appendix. Only summaries of the results for each configuration are presented here. BUOYANCY CHAMBER The tests using the cylindrical buoyancy chambers (figure 9) were the first runs made. The first step was to find a trap that worked well enough to be a starting point. This accounted for the large number of various configurations and few number of runs made at each pour rate. If a setup looked promising, work continued, but if it didn't, the idea was dropped. Testing was not continued to see "how bad" something was. For this reason, it is nearly impossible to show specifically how different variables affected performance. However, generalizations can be made. Having the inlet and exit passages on the same axis or using a top inlet, bottom exit gave poor performance for light inclusions. The flow did not slow down enough in the chamber to allow the inclusions time to separate. Efficiencies rarely got above 5096 (see runs ). These types of traps would probably work better in sand casting where the pour rates are much slower. The time and location that the inclusions are
35 28 introduced into the flow had a large effect on the efficiency of the inclusion trap. The pre-pour introduction gave the worst performance and resulted in all inclusions getting into the mold when no trapping devices were used. This is shown in runs in the appendix. As a result, it was decided to use this method for the majority of the tests. It was felt that if a device will separate the inclusions with this type of introduction, better with other later types of introduction. it would do It was also more consistent since it did not rely on a person's timing. The chamber did show some promise when the inlet and outlet passage were moved to opposite sides of the cylinder as shown in figure 13. Offsetting the inlet and outlet to each side of the chamber slowed the fluid down and removed a fair amount of inclusions. Figure 13. Buoyancy chamber with offset inlet and exit A datum to judge performance was made (runs )
36 29 using a 3.75" long buoyancy chamber with an offset inlet and exit. Other setups were tested against this. For each case, five runs were made, and both heavy (1.2 sg, 3mm acetate balls) and light (0.5 sg, 3mm wooden cubic beads) inclusions were used. Inclusion introduction was pre-pour (pp), meaning they were placed at the elbow at the bottom of the downsprue. Table I shows the separation efficiency (number of beads caught in separator divided by the number of beads caught plus the number that got through) for different pour rates and for both heavy and light inclusions. It can be seen that light inclusions were not as affected by pour rates as heavy ones. This was not the case for all devices (see swirl chambers). Table I. Effect of pour rate on heavy and light inclusion separation efficiency for a 3.5" dia. X 3.75" horizontal cylinder using buoyancy for separation. (runs ) slow med fast light inclusions heavy inclusions The cylinder length had a considerable effect on both heavy and light inclusions. This is obviously due to the fact that a longer cylinder gives more time for inclusions to be separated. Table II shows the performance of the 3.5" diameter cylindrical buoyancy chamber for various lengths.
37 30 Table II. Effect of cylinder length on heavy and light inclusion separation efficiency for a 3.5" dia. horizontal cylinder using buoyancy for separation. All pours medium speed. (runs , , ) light 3.75" long " long " long 6 10 heavy Putting an overflow choke on the exit of the cylinder increased the efficiency for both heavy and light inclusions. This is shown in table III. Again, this slows flow and gives inclusions longer to separate. Table III. Effect of overflow outlet choke on heavy and light inclusion separation efficiency for a 3.5" dia. X 3.75" horizontal cylinder using buoyancy for separation. (runs , ) All pours medium speed. light heavy no choke overflow outlet choke It was noticed that inclusions that got through the chamber lingered and swirled before going on to the mold. This led us to try a two chamber design that was made by placing a baffle in the original chamber. This is shown on figure 14.
38 " variable 1-4. \.: -..- Figure 14. Buoyancy cylinder with baffle Various locations of the baffle were tried. The design worked well with the inlet passage on top, the exit passage to one side, and the baffle one inch from the front with the opening down. The flow was dampened in the first chamber, then formed a swirl in the second chamber that would catch inclusions. The design didn't work well for faster pours and heavy inclusions, but did improve efficiency for light inclusions at slow pours. Table IV shows the efficiency of the cylinder with a baffle located one inch from the inlet compared to the cylinder without a baffle.
39 32 Table IV. Effect of internal baffle on heavy and light inclusion separation efficiency for a 3.5" dia. X 3.75" horizontal cylinder using buoyancy for separation. All pours medium speed. (runs , ) slow med fast light heavy with baffle, light with baffle, heavy SMALL SWIRL CHAMBERS Several arrangements of inlets and outlets were tried with the small swirl chamber. In all cases, having the exit passage above the inlet passage worked best. This seems wrong since the beads are lighter than the surrounding water and would tend to float. In reality the swirl was observed to form before the fluid level reached the outlet. For cases with the inlet above the outlet, the fluid fell and splashed as shown on figure 15. This turbulence kept the inclusions mixed and the swirl took longer to develop, allowing early inclusions to get through.
40 33 Mir1.5" dia 3.5" 1.125" dia entrance below exit "nice" swirl forms entrance above exit initial splashing and turbulence keep inclusions mixed Figure 15. Inlet vs. outlet location on swirl chamber The major sets of tests were plain swirl chambers swirl chambers with swirl chambers with swirl chambers with swirl chambers with swirl chambers with swirl chambers with 2" wells 2" extensions 2" caps inlet chokes exit chokes plugged vent holes optimum combinations Each configuration was tried with enough runs (usually five) to get a confident estimate of efficiency. All runs
41 were made with the inlet below the exit as described above. 34 For obviously poor setups, less runs were made. The raw data for all runs are in the appendix and a summary of the results is given table V. plotted in figures Some of the data have been
42 Table V. Summary of Results for Small Swirl Chambers 35 Efficiency Fill time Description plain swirl chamber Dia. S M F S M F swirl chamber with 2" well swirl chamber with 2" extension swirl chamber with 2" cap plain swirl chamber with outlet venturi choke plain swirl chamber with plugged vent hole
43 36 Table V continued. Summary of Results for Small Swirl Chambers Efficiency Fill time Description plain chamber with 50% choke inlet Dia. S M F S M F plain chamber with 75% choke inlet swirl chamber with 50% inlet choke and 2" well swirl chamber with 75% inlet choke and 2" well " well, 50% inlet choke, overflow exit choke
44 37 Table V continued. Summary of Results for Small Swirl Chambers Efficiency Fill time Description 75% inlet choke and venturi outlet choke 2" well, 50% inlet choke vertical position 2" well, 50% inlet choke tilted 45 degrees 2" well, 50% inlet choke horizontal position Dia. S M F S M F All setups shown were run with the inlet passage below the exit passage and with both inlet and exit stream flowing in the same angular direction. Both the overflow exit choke and the venturi exit choke had a flow area of 0.22 in"2, a reduction in area of 88%. Inlet tube = 1.5" I.D. Exit tube = 1.125" I.D.
45 38 Plain, wells, caps and extensions Increasing the time for the swirl to develop was done by either adding a well, cap or extension as shown in figure 16. Well DIAMETERS; 2.5", 3", 3.5" & 4" Cap Extension Figure 16. Small swirl chambers; plain, well, extension and cap
46 39 For all pour rates, the well performed better than the cap and the cap performed better than a plain swirl chamber. The effect of an extension seems to vary with pour rate. At slow pours (figure 17), the extension was equivalent to a plain chamber. This was because the plain chamber had adequate time for the swirl to form before the fluid left. As the pour rates increased (figure 18 & 19), the effectiveness of the extension over the plain chamber increased due to the swirl being able to develop better ao Chamber diameter (inches) Figure 17. Small swirl chamber efficiency for slow pour
47 r Chamber diameter (inches) 4.50 Figure 18. Small swirl chamber efficiency for medium pour WELL EXTENSION CAP PLAIN I I I I Chamber diameter (inches) Figure 19. Small swirl chamber efficiency for fast pour
48 The inlet area on some runs of the plain swirl chambers was choked 50% and 75% of full open as shown in figure The efficiencies of a plain swirl chamber with no inlet choke, 50% inlet choke and 75% inlet choke for various diameters are shown on figures for slow, medium and fast pours, respectively. The corresponding fill times are shown on figures for slow, medium and fast respectively. pours, The chokes slow the incoming fluid down and make the chamber diameter bigger compared to the inlet stream. Both the 50% IC (inlet choke) and 75% IC gave definite efficiency increases over the unchoked chamber. While the 50% IC improvement was usually not as great as the 75% IC, its corresponding decrease in fill time made it more desirable s0.00 to % INLET CHOKE 50% INLET CHOKE I PLAIN Chamber diameter (inches) 4.50 Figure 20. Efficiency of plain swirl chamber with inlet choke. Slow pour
49 , Chamber diameter (inches) Figure 21. Efficiency of plain swirl chamber with inlet choke. Medium pour I I Chamber diameter (inches) Figure 22. Efficiency of plain swirl chamber with inlet choke. Fast pour
50 X H.ET CHOKE NLET CI-OKE PLAN Chamber diameter (inches) Figure 23. Fill time of plain swirl chamber with inlet choke. Slow pour X NLET CHOKE g x X IMET CHOKE PLAN Chamber diameter (inches) Figure 24. Fill time of plain swirl chamber with inlet choke. Medium pour 0
51 44 Ms X TILET CHOKE MET CHOKE PLAIN K Chamber diameter (inches) Figure 25. Fill time of plain swirl chamber with inlet choke. Fast pour Table VI shows the effect of a venturi outlet choke. The use of an outlet choke on the plain swirl chambers gave highly improved efficiency, especially for fast pours. However, when used with the best setup (a 3.5" swirl chamber with a 2" well and 50% inlet choke) the improvement efficiency was small. in
52 45 Table VI. Effect of venturi outlet choke on separation efficiency for small swirl chambers Swirl chamber configuration Dia. Without outlet choke With outlet choke plain 2.5" 10,3,3 16,27,18 plain 3.0" 39,14,7 56,30,22 plain 3.5" 83,47,34 86,67,46 plain 4.0" 84,64,53 89,92,86 2" well, 50% IC 3.5" 99,91,89 97,95,90 One concern that PCC had was the long, narrow vent tube required to ventilate the swirl chamber. Because it was so narrow, it could be susceptible to breakage. They were interested in the performance of the swirl chamber when a vent was not used. When run without a vent hole, the plain swirl chambers actually seemed to give slightly better separation efficiency. However, the filling of the mold was unacceptable because the large pocket of air that would normally be vented ended up in the part cavity. Optimization Based on the above conclusions, the small swirl chambers were run with combinations of 2" wells, inlet chokes & exit chokes. The results for a swirl chamber with a 2" well and no outlet choke are shown in figures for slow, medium and fast pours, respectively. Each figure
53 46 gives the results for no inlet choke, a 50% inlet choke and a 75% inlet choke for various diameters. It can be seen from these figures that a 3.5" to 4.0" swirl chamber with a 2" well and 50% inlet choke gives very good separation, equaling with a faster fill time. one with a 75% inlet choke but ; INLET CHOKE 50; INLET CHORE WELL Chamber diameter (inches) 4.50 Figure 26. Efficiency of swirl chamber with inlet choke and 2" well. Slow pour
54 INLET CHOKE WELL I Chamber diameter (inches) 4.50 Figure 27. Efficiency of swirl chamber with inlet choke and 2" well. Medium pour Figure Chamber diameter (inches) Efficiency of swirl chamber with inlet choke and 2" well. Fast pour 4.50
55 48 Other inclusion tests A quantity of bubble alumina in three sizes was supplied by P.C.C. Each size consisted of both light (the alumina bubbles floated) and heavy (broken or deformed bubbles). The light bubble alumina was of the most interest, since it had a specific density around 0.85 which is heavier than the wood beads usually used (s.g ). Theoretically, they should be harder to separate, since their density is closer to the carrying medium. They are also much closer to the size that P.C.C. wanted studied (0.8 mm 1.8 mm, vs smallest beads 3 mm). P.C.0 also supplied sandblasting medium and silicon carbide particles which could be used to model heavy inclusions. In order to study these inclusions, a small gate valve that would not interfere with flow was placed between the chamber and part mold. A given quantity of bubble alumina was placed at the bottom of the downsprue and the run was made. Immediately afterwards, the valve was shut and the alumina was removed from the two parts of the mold with a filter and allowed to dry. A digital scale was used to measure the amounts of alumina. The video setup used to record the fills using beads was used for the alumina at first. However, due to the small size of the alumina and it's white color, a new
56 49 method was tried. This consisted of enclosing the mold, stand and crucible stand in black plastic and using blacklight (ultra-violet light). Some alumina was painted with fluorescent paint. When the run was viewed with the naked eye, the effect was quite impressive as the alumina bubbles glowed. Trying to capture this effect on video was less successful. The alumina wasn't nearly as bright, especially when the shutter speed was increased to reduce blur. An ultra-violet filter on the video camera lens gave the picture a much better overall quality, but seemed to decrease the brightness of the alumina. The tundish and part mold are slightly fluorescent themselves and the clear plastic being used filters some of the UV light leading to a lower quality picture. However, this method was definitely better than that previously used for tracking the smaller inclusions. Comparing each case with its corresponding results done with wooden beads showed that bubble alumina runs had lower efficiencies. For example a 3.5" swirl chamber with 2" well and 50% inlet choke had efficiencies of 99 %, 91% & 89% (slow, medium & fast pours) with the wooden bead inclusion models. The same setup using light bubble alumina inclusion models gave efficiencies of 96%, 90% & 78 %. The decrease in efficiency, especially for fast
57 50 pours, is probably due to the heavier inclusions. However, the performance was still quite good. Fluid velocity One concern expressed about the swirl chamber is that the fluid velocity at the wall may be too high and could erode the walls, contributing to more inclusions in the mold. A study was made to get an estimate to the fluid velocities in the downsprue and swirl chamber and how these compare. This was done by putting inclusions into the flow and assuming that they are moving at approximately the same speed as the fluid. The video equipment used takes one frame every 1/60 sec. By advancing the tape frame by frame and getting the displacements of the beads, estimate of the fluid velocity was made. an The swirl chamber tested was the 3" diameter with a 2" well. Both unchoked and 75% inlet choked were tried. Numerical results are shown in table VII. It should be remembered that these are very rough estimates and some simplifying assumptions were made (inclusions are moving as fast as the fluid, the swirl has a constant angular velocity everywhere). It can be seen that maximum velocities are approximately 10% chamber than in the downsprue. 20% higher in the swirl
58 51 Table VII. Fluid velocities in the 3" dia. swirl chamber with 2" well max velocity at bottom of downsprue unchoked 75% inlet choke slow pour 5 (fps) 5 medium pour 8 8 fast pour max velocity at swirl wall unchoked 75t choke inlet slow pour 6 (fps) 9 medium pour 9 11 fast pour CONICAL SWIRL CHAMBERS The results of the conical swirl chambers are shown in table VIII. Cone 1 (see figure 12) worked quite well with a 50% inlet choke and even better with an exit choke. This indicates that conical swirl chambers can work at least as well as the cylindrical shaped ones. One problem with studying the cones was their difficulty in casting. This made investigating many different cone geometries unfeasible.
59 52 Table VIII. Summary of Results for Conical Swirl Chambers Description Efficiency Fill time cone #1, upper inlet cone #1, lower inlet cone #1, lower inlet, 50% inlet choke cone #1, lower inlet, 50% inlet choke, overflow outlet choke cone #1, lower inlet, 50% inlet choke, sideflow outlet choke cone #2, radial outlet LARGE SWIRL CHAMBER A summary of the results for the large swirl chamber is given in table IX. During work with the small swirl chambers, it was found that a 3.5" swirl chamber with a 50% inlet choke and a well gave very good results, 99% (slow), 91% (medium) and 89% (fast). A larger 8" dia chamber with a 50% IC and well gave similar good results, 90%, 88% & 88%.
60 Table IX. Summary of Results for Large Swirl Chamber 53 RTA PWCE IC OC CN Description S M F R P R P X R W R W X R W X C R W C R W X X W X X C R P X X C R P X C R C X C R W X C T W X T W X C T W X X C T W X X T P X X T P X X Cl T P X A P X A W X A W X C A W X X C A W X X A W X X C A P X X A P X X C
61 Table IX continued. Summary of Results for Large Swirl Chamber 54 RTA PWCE IC OC CN Description S M F R W X top outer cone (4 lbs clay) R W X C2 top outer cone (4 lbs clay) R P X top outer cone (4 lbs clay) R W X full outer cone (8 lbs clay) R W X X full outer cone (8 lbs clay) R E X full outer cone (12 lbs clay) R E X X full outer cone (12 lbs clay) R E X R E X X R E X X top outer cone (4 lbs clay) R E X top outer cone (4 lbs clay) R E X C R E X X C R W X top outer cone (4 lbs clay)-late inc R W X late inclusions A W X top outer cone (4 lbs clay) T W X top outer cone (4 lbs clay)
62 Table IX continued. Summary of Results for Large Swirl Chamber 55 RTA PWCE IC OC CN Description S M F R W X C2* ice cream cone R W X C2* ice cream cone-late inclusions R W X C2* ice cream cone-heavy inclusions RTA; radial, tangential or anti-tangential outlet PWCE; plain, well, cap or extension IC; 50% inlet choke OC; overflow outlet choke IN; insert used. C1 = "stubby" cone, C2 = "pointy" cone, C2* = inverted poiny cone
63 56 Table X compares the results for different configurations of radial, tangential and anti-tangential outlets (see figure 29). In general, the trend seems to be anti-tangential and radial outlets are about equal and better than tangential outlets. This doesn't seem intuitive since tangential outlets will lead to a stronger swirl. But they let the fluid out quicker, giving the earlier inclusions less time to be separated. radial tangential anti-tangential Figure 29. Radial, tangential and anti-tangential outlets